## Absence of internal conical refraction with the spatially dispersive index surface of fluorine; discussion of the orthogonality of the Poynting vector to the index surface

Optics Express, Vol. 14, Issue 8, pp. 3339-3344 (2006)

http://dx.doi.org/10.1364/OE.14.003339

Acrobat PDF (93 KB)

### Abstract

Since 2001 the intrinsic birefringence of fluorine has been accessible to experiment. It is known that its intrinsic anisotropy is entirely due to spatial dispersion, and that the index surface of fluorine and crystals with the same symmetry has seven optical axes, four of them intersecting this surface at pairs of conical points. I point out the fact that there is no internal conical refraction, but only simple refraction (and without walk-off), with these conical points. I also explain why the rays are not *a priori* normal to the index surface in the case of fluorine because of its spatial dispersion; and I discuss two particular cases of spatial dispersion where the Poynting vector remains orthogonal to the index surface.

© 2006 Optical Society of America

## 1. Introduction

_{2}. Its crystal having cubic symmetry, it was thought that no intrinsic birefringence occurs: such crystals can be neither uniaxial nor biaxial. But this property is based upon the simplifying assumption that the material is local [1]; that approximation ends up loosing its validity when the wavelength to crystal unit cell ratio

*λ*/

*a*decreases below a certain point [2

2. V. L. Ginzburg, “On crystal optics with spatial dispersion,” Physics reports **194**, 245–251 (1990). [CrossRef]

*ω*and wave vector noted

**q**(instead of

**k**, according to the recent quoted papers of Burnett and al.), the non-locality of a dielectric is easily described by the dependence of its electric permittivity tensor (

*ε*) with

**q**: this phenomenon is also called “spatial dispersion”, and adds to the usual dispersion described by the dependence of (

*ε*) with

*ω*. Any material shows some absorption, and for a dielectric it means that (

*ε*) is not Hermitian, according to the Kramers-Kronig relations involving its usual dispersion. But when a medium is considered being transparent the effects of the anti-Hermitian part of (

*ε*) are essentially negligible - and with fluorine in the optical domain this is the case over an exceptionally broad band going from thermal infrared to vacuum ultraviolet (9-0.12 μm approximately); so in this work we shall consider only Hermitian permittivity tensors and real wave vectors. In the visible domain, ∥

**q**∥ is small enough compared to 1/

*a*for (

*ε*) (

*ω*,

**q**) to be nearly equal to (

*ε*) (

*ω*, 0) which is scalar for crystals having cubic symmetry, so that they seem isotropic. But that is not true in the vacuum ultraviolet, so a new form of anisotropy occurs: the intrinsic birefringence by spatial dispersion. That phenomenon has been predicted by Lorentz in 1878 [3], theoretically studied by Agranovitch and Ginzburg and experimentally observed in non-optical materials since 1960 [4], then recently rediscovered in fluorine where it complicates the design of lithography objectives [5

5. J. H. Burnett, Z. H. Levine, and E. L. Shirley, “Intrinsic birefringence in calcium fluoride and barium fluoride,” Phys. Rev. B **64**, 241102(R) (2001). [CrossRef]

*ε*) (

*ω*,

**q**) is given by its second order expansion for

*a*∥

**q**∥ ≪1. For crystal of classes

*T*

_{d}and

*O*

_{h}, (in Schoenflies notation, fluorine being of class

*ε*)(

*ω*,

**q**) - in an orthonormal basis whose unit vectors

**x̂**,

**ŷ**and

**ẑ**are parallel to the edges (

*E*) of the cubic conventional unit cell (

*C*) - are given by [4]

*ε*

_{0}denotes the electric permittivity of the vacuum,

*j*and

*l*are equal to 1, 2, and 3 for axes

*x*,

*y*, and

*z*respectively. Among the parameters

*n*

_{0},

*α*,

*β*and

*γ*, only the latter is responsible for a dielectric anisotropy: if

*γ*= 0 , the refractive index

*n*of the spatially dispersive medium has its isotropic value [6]

*q*

_{0}is the modulus of wave vectors in a vacuum for the given frequency) ; Eq. (2) results from the two Maxwell curl Eqs., which yield

*n*.

*α*is not involved in Eq. (2) for

*γ*= 0 because one verifies straightforwardly that the electric field

**E**is parallel to the electric displacement

**D**(a fact which will be useful later) hence

**E**is transverse. For such crystals with

*γ*≠ 0 , the study of the index surface [7

7. J. H. Burnett, Z. H. Levine, E. L. Shirley, and J. H. Bruning, “Symmetry of spatial-dispersion-induced birefringence and its implications for CaF_{2} ultraviolet optics,” J. Microlith., Microfab., Microsyst. **1**, 213–224 (2002). [CrossRef]

*D*) of (

*C*). One should note that its other three optical axes, those parallel to (

*E*), are not associated to conical points (like for conventional uniaxial crystals).

*i*.

*e*. for which

**B**=

*μ*

**H**where its magnetic permeability is a real constant

*μ*,

**B**and

**H**being the magnetic induction and field), when wave vector

**q**is parallel to an optical axis, any transverse direction is allowed for

**D**, and (

**D**,

**H**,

**q**) forms an orthogonal triplet. Generally there is a “walk-off angle”

*χ*= (

**D**,

**E**), so that the direction of the Poynting vector

**R**≡

**E**×

**H**makes with

**q**the same angle

*χ*which depends on the

**D**-direction - because (

**E**,

**H**,

**R**) forms another orthogonal triplet [8].

*χ*= 0 if

**q**is parallel to it.

**q**is parallel to one of them

*χ*= 0 only for

**D**normal to the plane of these axes but

*χ*differs from zero for all other directions allowed for

**D**, so that the set of refracted rays associated to one incident non polarized ray in that case forms a cone. That well-known phenomenon of internal conical refraction is geometrically understood by use of the classical property that the Poynting vector is orthogonal to the index surface at its point associated to the wave vector [9].

**q**is parallel to an optical axis is general. But is conical refraction possible in fluorine?

## 2. Absence of internal conical refraction in fluorine

**q**is parallel to (

*E*), the polarization properties of

**D**and

**E**are the same as in an uniaxial crystal with

**q**parallel to its optical axis:

*χ*= 0 for all the directions allowed for

**D**, so there is no internal conical refraction, and there is no conical point associated to this optical axis on the index surface [7

7. J. H. Burnett, Z. H. Levine, E. L. Shirley, and J. H. Bruning, “Symmetry of spatial-dispersion-induced birefringence and its implications for CaF_{2} ultraviolet optics,” J. Microlith., Microfab., Microsyst. **1**, 213–224 (2002). [CrossRef]

**q**is parallel to (

*D*). In that case relation (1) becomes

*ε*) has the same structure as the permittivity tensor of an isotropic spatially dispersive medium, satisfying relation (2) where

*β*is replaced by

**D**components on the crystallographic axes). For our purpose, the important consequence is that

**E**is parallel to

**D**here (like in the case leading to Eq. (2)) - in other terms, one easily sees that ⌊11̅0⌋ and ⌊112̅⌋ are two eigenvectors, not only of the projection (

*ε*

^{-1})

_{⊥}of (

*ε*

^{-1}) - the inverse of the permittivity (used by [7

7. J. H. Burnett, Z. H. Levine, E. L. Shirley, and J. H. Bruning, “Symmetry of spatial-dispersion-induced birefringence and its implications for CaF_{2} ultraviolet optics,” J. Microlith., Microfab., Microsyst. **1**, 213–224 (2002). [CrossRef]

**q**, but also of the whole tensor (

*ε*

^{-1}) and of (

*ε*) given by Eq. (4). Therefore

*χ*= 0, hence

**R**is again parallel to

**q**for all the directions allowed for

**D**, and there is no internal conical refraction.

*D*) [7

_{2} ultraviolet optics,” J. Microlith., Microfab., Microsyst. **1**, 213–224 (2002). [CrossRef]

**R**to the index surface no longer holds for crystal showing spatial dispersion.

## 3. Discussion of the orthogonality of the Poynting vector to the index surface

### 3.1 General case of a linear spatially dispersive dielectric

*ε*) is entirely due to spatial dispersion. Hence, the scalar product of both sides of Eq. (9) by

**E̲**

^{*}, subtracted from the scalar product of (8) by

**H̲**

^{*}, gives

**R**〉 is the mean value of the Poynting vector. Up to now, the wave vector

**q**could in fact be complex (case of an absorbing medium, or of an evanescent wave, etc.); but we want to consider that a point of the index surface suffices to determine completely

**q**, so we restrict ourselves to the case where

**q**is real, hence we consider that the medium is transparent. This leads to a new simplification, because with

**q**real Eq. (6) gives

*ε*)+ denotes the Hermitian conjugate of (

*ε*), and (

*ε*)

^{ah}its anti-Hermitian part. We know that for a transparent medium, (

*ε*) is not automatically real (it is complex when the spatial dispersion involves gyrotropy), but it is always Hermitian, hence (

*ε*)

^{ah}is null [11] and finally

*ε*) is null and for a given

**q**all the directions of the infinitesimal vectors d

**q**span the tangent plane of the index surface at its point associated to

**q**, so 〈

**R**〉 is perpendicular to that surface at this point (let us note that this result holds also if the magnetic permeability is a Hermitian matrix independent of

**q**).

**R**〉 is not always perpendicular to that surface; this is possible because the medium is spatially dispersive then (d

*ε*) is not null.

*ε*) is not null but

**E̲**

^{*}.(d

*ε*)

**E̲**is null for each

**q**, hence 〈

**R**〉 is always perpendicular to their index surface; I shall point out two such cases.

### 3.2 Particular case of a purely gyrotropic medium

*ε*)(

*ω*,

**q**) to its first order in

**q**; then [2

2. V. L. Ginzburg, “On crystal optics with spatial dispersion,” Physics reports **194**, 245–251 (1990). [CrossRef]

*i*

^{2}= -1, and

*j*= 1,

*l*= 2,

*m*= 3, and any even permutation

*p*are real. But it is well-known that, in such a case ([10] pp. 433–434),

**E**and

**D**are always parallel (their two eigenvibrations being left and right-handed circularly polarized), the index surface is composed of two spheres centered at the origin; then

**R**and

**q**are always parallel, and

**R**is normal to the index surface, although (d

*ε*) is not null! This is possible because here

**E̲**×

**E̲**

^{*}is parallel to

**q**(

**E̲**and

**E̲**

^{*}being transverse like

**D**), d

**q**is orthogonal to

**q**because of the form of the index surface, hence

### 3.3 Particular case of a spatially dispersive non gyrotropic medium

*γ*= 0 ; moreover, its index surface is a sphere of radius

*n*

_{i}given by relation (2), and

**E̲**is orthogonal to

**q**. In this case, we find

**E̲**.

**q**,

**E̲**

^{*}.

**q**and

**q**.d

**q**are null.

## 4. Conclusion

**q**parallel to any of the seven optical axes of the fluorine, there is neither double nor internal conical refraction, only a simple refraction and without walk-off - the refractive index of the crystal being given by relation (5). This may in fact simplify the correction of the birefringence of fluorine in photolithography objectives, because one way used to correct it is to combine fluorine lenses whose geometrical axes are parallel to (

*D*), the transverse crystal axes being rotated by odd multiples of 60° from a lens to the following one [7

_{2} ultraviolet optics,” J. Microlith., Microfab., Microsyst. **1**, 213–224 (2002). [CrossRef]

## Acknowledgments

## References and links

1. | J. D. Jackson, |

2. | V. L. Ginzburg, “On crystal optics with spatial dispersion,” Physics reports |

3. | H. A. Lorentz, |

4. | V. M. Agranovich and V. L. Ginzburg, |

5. | J. H. Burnett, Z. H. Levine, and E. L. Shirley, “Intrinsic birefringence in calcium fluoride and barium fluoride,” Phys. Rev. B |

6. | L. Dettwiller, “Observation récente d’une forme de biréfringence dans certains cristaux à symétrie cubique: théorie et conséquences pratiques,” Bull. Un. Prof. Phys. Chim. |

7. | J. H. Burnett, Z. H. Levine, E. L. Shirley, and J. H. Bruning, “Symmetry of spatial-dispersion-induced birefringence and its implications for CaF |

8. | M. Born and E. Wolf, |

9. | G. Bruhat, |

10. |
see for example
L. Landau and E. Lifchitz, |

11. | L. Dettwiller, “Propagation de la lumière, dispersion et absorption”, in |

12. | L. Dettwiller, “Propriétés inédites de la biréfringence des cristaux à symétrie cubique du type de la fluorine,” presented at Horizons de l’Optique 2005, Chambéry, France, 8-10 Nov. 2005 |

**OCIS Codes**

(160.1190) Materials : Anisotropic optical materials

(160.4760) Materials : Optical properties

(260.1440) Physical optics : Birefringence

(260.5430) Physical optics : Polarization

**ToC Category:**

Materials

**History**

Original Manuscript: October 27, 2005

Revised Manuscript: April 3, 2006

Manuscript Accepted: April 7, 2006

Published: April 17, 2006

**Citation**

Luc Dettwiller, "Absence of internal conical refraction with the spatially dispersive index surface of fluorine; discussion of the orthogonality of the Poynting vector to the index surface," Opt. Express **14**, 3339-3344 (2006)

http://www.opticsinfobase.org/oe/abstract.cfm?URI=oe-14-8-3339

Sort: Year | Journal | Reset

### References

- J. D. Jackson, Classical Electrodynamics, 2nd edition (Wiley, New York, 1975): pp. 14-16.
- V. L. Ginzburg, "On crystal optics with spatial dispersion," Physics reports 194, 245-251 (1990). [CrossRef]
- H. A. Lorentz, Collected papers, Vol. II (Martinus Nijohff, The Hague, 1936): p. 79.
- V. M. Agranovich and V. L. Ginzburg, Crystal Optics with Spatial Dispersion, and Excitons, 2nd edition, Solid-State Science vol. 42 (Springer, Berlin, 1984).
- J. H. Burnett, Z. H. Levine and E. L. Shirley, "Intrinsic birefringence in calcium fluoride and barium fluoride," Phys. Rev. B 64, 241102(R) (2001). [CrossRef]
- L. Dettwiller, "Observation récente d’une forme de biréfringence dans certains cristaux à symétrie cubique: théorie et conséquences pratiques," Bull. Un. Prof. Phys. Chim. 99 (2), 77-103 (2005).
- J. H. Burnett, Z. H. Levine, E. L. Shirley and J. H. Bruning, "Symmetry of spatial-dispersion-induced birefringence and its implications for CaF2 ultraviolet optics," J. Microlith., Microfab., Microsyst. 1, 213-224 (2002). [CrossRef]
- M. Born and E. Wolf, Principles of optics - Electromagnetic theory of propagation interference and diffraction of light (Pergamon, Oxford, 1980): p. 668.
- G. Bruhat, Cours de physique générale - Optique (Masson, Paris, 1992): pp. 462-463.
- see for example L. Landau and E. Lifchitz, Physique théorique - tome 8 - Électrodynamique des milieux continus (Mir, Moscou, 1969).
- L. Dettwiller, "Propagation de la lumière, dispersion et absorption", in EGEM, Optique géométrique et propagation, J.-L. meyzonnette ed. (Hermès Lavoisier, Paris, 2003): pp. 63-64.
- <other>. L. Dettwiller, "Propriétés inédites de la biréfringence des cristaux à symétrie cubique du type de la fluorine," presented at Horizons de l’Optique 2005, Chambéry, France, 8-10 Nov. 2005 </other>

## Cited By |
Alert me when this paper is cited |

OSA is able to provide readers links to articles that cite this paper by participating in CrossRef's Cited-By Linking service. CrossRef includes content from more than 3000 publishers and societies. In addition to listing OSA journal articles that cite this paper, citing articles from other participating publishers will also be listed.

« Previous Article | Next Article »

OSA is a member of CrossRef.